LMucko/crystallography-open-database huggingface dataset:
Halite-sylvite thermoelasticity Sample: r57733, T = 500 C, P = 15.0 kbar, cell volume = 241.68 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003135
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r57733, T = 500 C, P = 15.0 kbar, cell volume = 241.68 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     KCl
_chemical_formula_sum            'Cl K'
_chemical_name_mineral           Sylvite
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.2289
_cell_length_b                   6.2289
_cell_length_c                   6.2289
_cell_formula_units_Z            4
_cell_volume                     241.676
_database_code_amcsd             0003224
_diffrn_ambient_pressure         1.5e+06
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    2.049
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        'K Cl'
_cod_database_code               9003135
Halite-sylvite thermoelasticity Sample: r57717, T = 500 C, P = 17.1 kbar, cell volume = 239.78 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003136
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r57717, T = 500 C, P = 17.1 kbar, cell volume = 239.78 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     KCl
_chemical_formula_sum            'Cl K'
_chemical_name_mineral           Sylvite
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.2126
_cell_length_b                   6.2126
_cell_length_c                   6.2126
_cell_formula_units_Z            4
_cell_volume                     239.784
_database_code_amcsd             0003225
_diffrn_ambient_pressure         1.71e+06
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    2.065
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        'K Cl'
_cod_database_code               9003136
Halite-sylvite thermoelasticity Sample: msl515037, T = 600 C, P = 0.0 kbar, cell volume = 270.14 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003137
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: msl515037, T = 600 C, P = 0.0 kbar, cell volume = 270.14 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     KCl
_chemical_formula_sum            'Cl K'
_chemical_name_mineral           Sylvite
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.4644
_cell_length_b                   6.4644
_cell_length_c                   6.4644
_cell_formula_units_Z            4
_cell_volume                     270.137
_database_code_amcsd             0003226
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    1.833
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        'K Cl'
_cod_database_code               9003137
Halite-sylvite thermoelasticity Sample: r57781, T = 600 C, P = 9.9 kbar, cell volume = 251.14 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003138
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r57781, T = 600 C, P = 9.9 kbar, cell volume = 251.14 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     KCl
_chemical_formula_sum            'Cl K'
_chemical_name_mineral           Sylvite
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.3092
_cell_length_b                   6.3092
_cell_length_c                   6.3092
_cell_formula_units_Z            4
_cell_volume                     251.144
_database_code_amcsd             0003227
_diffrn_ambient_pressure         9.9e+05
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    1.972
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        'K Cl'
_cod_database_code               9003138
Halite-sylvite thermoelasticity Sample: r57721, T = 600 C, P = 17.3 kbar, cell volume = 242.28 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003139
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r57721, T = 600 C, P = 17.3 kbar, cell volume = 242.28 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     KCl
_chemical_formula_sum            'Cl K'
_chemical_name_mineral           Sylvite
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.2341
_cell_length_b                   6.2341
_cell_length_c                   6.2341
_cell_formula_units_Z            4
_cell_volume                     242.282
_database_code_amcsd             0003228
_diffrn_ambient_pressure         1.73e+06
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    2.044
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        'K Cl'
_cod_database_code               9003139
Halite-sylvite thermoelasticity Sample: r57725, T = 600 C, P = 17.3 kbar, cell volume = 241.59 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003140
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r57725, T = 600 C, P = 17.3 kbar, cell volume = 241.59 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     KCl
_chemical_formula_sum            'Cl K'
_chemical_name_mineral           Sylvite
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.2282
_cell_length_b                   6.2282
_cell_length_c                   6.2282
_cell_formula_units_Z            4
_cell_volume                     241.595
_database_code_amcsd             0003229
_diffrn_ambient_pressure         1.73e+06
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    2.050
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        'K Cl'
_cod_database_code               9003140
Halite-sylvite thermoelasticity Sample: b&w, T = 25 C, P = 0.0 kbar, cell volume = 242.35 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003141
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: b&w, T = 25 C, P = 0.0 kbar, cell volume = 242.35 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.9Na.1)Cl
_chemical_formula_sum            'Cl K0.9 Na0.1'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.2347
_cell_length_b                   6.2347
_cell_length_c                   6.2347
_cell_volume                     242.352
_cell_formula_units_Z            4
_database_code_amcsd             0003230
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      298.15
_exptl_crystal_density_diffrn    1.999
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.9 Na.1) Cl'
_cod_database_code               9003141
_amcsd_formula_title             (K.9Na.1)Cl
Halite-sylvite thermoelasticity Sample: als3k90, T = 500 C, P = 0.0 kbar, cell volume = 257.91 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003142
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als3k90, T = 500 C, P = 0.0 kbar, cell volume = 257.91 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.9Na.1)Cl
_chemical_formula_sum            'Cl K0.9 Na0.1'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.3654
_cell_length_b                   6.3654
_cell_length_c                   6.3654
_cell_volume                     257.915
_cell_formula_units_Z            4
_database_code_amcsd             0003231
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    1.878
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.9 Na.1) Cl'
_cod_database_code               9003142
_amcsd_formula_title             (K.9Na.1)Cl
Halite-sylvite thermoelasticity Sample: als2k90, T = 600 C, P = 0.0 kbar, cell volume = 262.49 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003143
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als2k90, T = 600 C, P = 0.0 kbar, cell volume = 262.49 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.9Na.1)Cl
_chemical_formula_sum            'Cl K0.9 Na0.1'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.4028
_cell_length_b                   6.4028
_cell_length_c                   6.4028
_cell_volume                     262.488
_cell_formula_units_Z            4
_database_code_amcsd             0003232
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    1.846
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.9 Na.1) Cl'
_cod_database_code               9003143
_amcsd_formula_title             (K.9Na.1)Cl
Halite-sylvite thermoelasticity Sample: b&w, T = 23 C, P = 0.0 kbar, cell volume = 236.48 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003144
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: b&w, T = 23 C, P = 0.0 kbar, cell volume = 236.48 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.1839
_cell_length_b                   6.1839
_cell_length_c                   6.1839
_cell_volume                     236.476
_cell_formula_units_Z            4
_database_code_amcsd             0003233
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      296.15
_exptl_crystal_density_diffrn    2.004
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003144
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: als11k80, T = 300 C, P = 0.0 kbar, cell volume = 244.34 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003145
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als11k80, T = 300 C, P = 0.0 kbar, cell volume = 244.34 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.2517
_cell_length_b                   6.2517
_cell_length_c                   6.2517
_cell_volume                     244.340
_cell_formula_units_Z            4
_database_code_amcsd             0003234
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      573.15
_exptl_crystal_density_diffrn    1.939
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003145
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: r55633, T = 300 C, P = 3.6 kbar, cell volume = 239.48 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003146
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r55633, T = 300 C, P = 3.6 kbar, cell volume = 239.48 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.2100
_cell_length_b                   6.2100
_cell_length_c                   6.2100
_cell_volume                     239.483
_cell_formula_units_Z            4
_database_code_amcsd             0003235
_diffrn_ambient_pressure         3.6e+05
_diffrn_ambient_temperature      573.15
_exptl_crystal_density_diffrn    1.978
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003146
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: als10k80, T = 350 C, P = 0.0 kbar, cell volume = 245.83 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003147
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als10k80, T = 350 C, P = 0.0 kbar, cell volume = 245.83 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.2644
_cell_length_b                   6.2644
_cell_length_c                   6.2644
_cell_volume                     245.832
_cell_formula_units_Z            4
_database_code_amcsd             0003236
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      623.15
_exptl_crystal_density_diffrn    1.927
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003147
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: r55501, T = 350 C, P = 17.2 kbar, cell volume = 224.31 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003148
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r55501, T = 350 C, P = 17.2 kbar, cell volume = 224.31 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.0760
_cell_length_b                   6.0760
_cell_length_c                   6.0760
_cell_volume                     224.312
_cell_formula_units_Z            4
_database_code_amcsd             0003237
_diffrn_ambient_pressure         1.72e+06
_diffrn_ambient_temperature      623.15
_exptl_crystal_density_diffrn    2.112
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003148
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: als9k80, T = 400 C, P = 0.0 kbar, cell volume = 247.44 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003149
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als9k80, T = 400 C, P = 0.0 kbar, cell volume = 247.44 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.2780
_cell_length_b                   6.2780
_cell_length_c                   6.2780
_cell_volume                     247.437
_cell_formula_units_Z            4
_database_code_amcsd             0003238
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      673.15
_exptl_crystal_density_diffrn    1.915
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003149
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: r55629, T = 400 C, P = 5.2 kbar, cell volume = 240.28 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003150
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r55629, T = 400 C, P = 5.2 kbar, cell volume = 240.28 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.2169
_cell_length_b                   6.2169
_cell_length_c                   6.2169
_cell_volume                     240.282
_cell_formula_units_Z            4
_database_code_amcsd             0003239
_diffrn_ambient_pressure         5.2e+05
_diffrn_ambient_temperature      673.15
_exptl_crystal_density_diffrn    1.972
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003150
Halite-sylvite thermoelasticity Sample: r55493, T = 450 C, P = 19.0 kbar, cell volume = 224.28 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003151
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r55493, T = 450 C, P = 19.0 kbar, cell volume = 224.28 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.0757
_cell_length_b                   6.0757
_cell_length_c                   6.0757
_cell_volume                     224.279
_cell_formula_units_Z            4
_database_code_amcsd             0003240
_diffrn_ambient_pressure         1.9e+06
_diffrn_ambient_temperature      723.15
_exptl_crystal_density_diffrn    2.112
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003151
_amcsd_formula_title             (K.8Na.2)Cl